Send Orders for Reprints to [email protected]
The Open Dentistry Journal, 2016, 10, 58-68
The Open Dentistry Journal Content list available at: www.benthamopen.com/TODENTJ/ DOI: 10.2174/1874210601610010058
Effect of Zirconia and Alumina Fillers on the Microstructure and Mechanical Strength of Dental Glass Ionomer Cements Júlio C. M. Souza1,2,*, Joel B. Silva3, Andrea Aladim4, Oscar Carvalho1, Rubens M. Nascimento2, Filipe S. Silva1, Antonio E. Martinelli4 and Bruno Henriques1,2,5,* 1
Center for Microelectromechanical Systems (CMEMS)-Uminho, Universidade do Minho, P-4800-058, Guimarães, Portugal 2 Post-Graduation Program in Dentistry (PPGO), Edif. CCS, School of Dentistry, Universidade Federal de Santa Catarina (UFSC), 88040-900, Florianópolis/SC, Brazil 3 School of Dentistry, School of Health Sciences (FCS), Universidade Fernando Pessoa (UFP), Porto, Portugal 4 Department of Materials Engineering, Universidade Federal do Rio Grande do Norte (UFRN), 59072-970, Natal/RN, Brazil 5 Ceramic and Composite Materials Research Group (CERMAT), Universidade Federal de Santa Catarina (UFSC), Campus Trindade, Florianópolis/SC, Brazil Abstract: Background: Glass-ionomer cements perform a protective effect on the dentin-pulp complex considering the F ions release and chemical bonding to the dental structures. On the other hand, those materials have poor physic-mechanical properties in comparison with the restorative resin composite. The main aim of this work was to evaluate the influence of zirconia and/or alumina fillers on the microstructure and strength of a resin modified glass-ionomer cement after thermal cycling. Methods: An in vitro experimental study was carried out on 9 groups (n = 10) of cylindrical samples (6 x 4 mm) made from resin modified glass-ionomer (Vitremer, 3M, USA) with different contents of alumina and/or zirconia fillers. A nano-hybrid resin composite was tested as a control group. Samples were mechanically characterized by axial compressive tests and electron scanning microscopy (SEM) coupled to energy dispersive X-ray spectrophotometry (EDS), before and after thermal cycling. Thermal cycling procedures were performed at 3000, 6000 and 10000 cycles in Fusayama´s artificial saliva at 5 and 60 oC. Results: An improvement of compressive strength was noticed on glass-ionomer reinforced with alumina fillers in comparison with the commercial glass ionomer. SEM images revealed the morphology and distribution of alumina or zirconia in the microstructure of glass-ionomers. Also, defects such as cracks and pores were detected on the glass-ionomer cements. The materials tested were not affected by thermal cycling in artificial saliva. Conclusion: Addition of inorganic particles at nano-scale such as alumina can increase the mechanical properties of glass-ionomer cements. However, the presence of cracks and pores present in glass-ionomer can negatively affect the mechanical properties of the material because they are areas of stress concentration. Keywords: Alumina, glass-ionomer cement, strength, thermal cycling, zirconia. * Address correspondence to these authors at the Post-Graduation Program in Dentistry (PPGO), School of Dentistry Universidade Federal de Santa Catarina (UFSC) Campus Trindade, Edif. CCS, 88040-900 Florianópolis/SC, Brazil; Email: [email protected]
2016 Bentham Open
Effect of Zirconia and Alumina Fillers
The Open Dentistry Journal, 2016, Volume 10 59
1. INTRODUCTION In dental practice, glass-ionomer cements are commonly used for dental restorations, preventive sealing of occlusal fissures or cementing prosthetic structures. However, the mechanical strength of glass-ionomer cements is low for posterior teeth areas in the oral cavity. Thus, technological developments are in progress to improve their properties leading to the modification of the chemical composition of those materials by adding inorganic reinforcement particles or resin monomers [1 - 3]. Glass ionomer cement (GIC) is the generic name for a group of classifying materials originally produced from glass calcium fluoro-aluminosilicate powder mixed with an aqueous solution of alkenoic acids [3, 4]. The powder of the ionomer glass is formed by fusion of its main components (SiO2, Al2O3 and CaF2) at a temperature between 1100 and 1500 °C to form a homogeneous calcium fluoro-aluminosilicate glass [4, 5]. Silica and alumina are responsible for the mechanical strength of the material while calcium fluoride will contribute to F ions release at the surrounding media [6, 7]. Additionally, the material properties of GIC are dependent on the type of alkenoic acid selected by the manufacturer. There is a consensus that high molecular weight acids increase the mechanical strength of the cement although they increase the viscosity of the bulk material [7, 8]. Also, the carboxylic groups present in the acidic liquid are responsible for the chemical adhesion of the material to the dental structures . The major disadvantages of glass ionomers are their low mechanical strength and high occlusal wear rate when compared to recent amalgam or resin composites [4, 6, 9]. For instance, a laminating technique involving resin composite coating the glass ionomer base is applied to associate high mechanical strength, chemical adhesion to tooth structures and release of F ions. Resin composites are materials with higher strength and resistance to wear compared to GIC. In these circumstances,GIC acts as a base or liner which is protected against surface wear and chewing forces as they are provided for posterior restorations [4, 10]. The cements modified by metallic fillers emerged from the original idea of adding silver alloy fillers into the generic GIC composition [8, 9]. The conventional ionomer cements modified by the addition of light-cured resin monomers (hydroxyethyl methacrylate) are commonly classified as resin-modified glass ionomer cements [4, 5, 8]. Modification of glass ionomer cement adding resin content has improved its mechanical and optical properties [1 - 3, 8]. Considering the previous pathways to improve strength by modifying the composition of the materials, the aim of this study was to evaluate the influence of the addition of zirconia and alumina fillers on the microstructure and mechanical strength of modified resin glass ionomer cements after thermal cycling. 2. MATERIALS AND METHODS 2.1. Synthesis of the Modified Glass-ionomer In this study, commercial resin-modified glass ionomer cement (GIC) (Vitremer, 3M, ESPE), named as VT , was used to synthesize a novel reinforced glass ionomer containing fillers based on yttria stabilized zirconia (SigmaAldrich) and aluminum oxide (Sigma- Aldrich), named as VTZ and VTA respectively from now on. The commercial GIC (VT) was mixed in a ratio of 2.68 g/ml on a glass plate and injected into a polytetrafluoroethylene mold using a Mark II Snap-fit syringe (Centrix, USA) (Fig. 1). The matrix had a capacity to produce six cylindrical samples (6 x 4 mm) simultaneously. The samples were covered with an acetate tape during the light-curing for 40 s using a Coltolux 75 (Coltène/Whaledent, Altstätten, Switzerland) cure device (Fig. 1C). The samples were produced by a single operator according to the manufacturer's recommendations. Reinforced GIC (VT) formulations were prepared by adding different amounts of zirconia (VTZ) and/or alumina (VTA) nano-fillers into the commercial GIC (VT) composition (Table 1). The cylindrical specimens of the reinforced GIC were prepared following the same method described for the commercial GIC (VT). A resin composite nano-hybrid (Great, VOCO; Germany), named GD from now on, was used in order to establish terms of comparison with the GIC (VT) tested . The cylindrical composite samples were prepared according to the manufacturer's instructions. A total of 210 cylindrical specimens were synthesized and divided into 9 groups (Table 1). 2.2. Mechanical Strength At first, 90 specimens were evaluated by compressive tests (n = 10) before thermal cycling tests. Then, 5 groups
60 The Open Dentistry Journal, 2016, Volume 10
Souza et al.
(VT, VTA, VTZ, VTZA and GD) consisting of a total of 120 samples were assessed by compressive tests before and after thermal cycling. Compressive tests were performed at 25 °C by using a universal mechanical testing machine (Instron 8874, MA, USA) with a 25 kN load cell. The tests were monitored using the Trapezium software. Test were carried out at a speed of 1 mm/min. A number of 10 specimens of each condition were tested in order to obtain mean values of the compressive force.
Fig. (1). (A) Polytetrafluoroethylene mold and (B) Mark II Snap-fit syringe. (C) Light-curing of (D) the cylindrical specimens.
2.3. Thermal Cycling Thermal cycling is an experimental method of simulating the effect of temperature variations on restorative materials as found in the oral cavity . For thermal cycling, the samples were immersed in two consecutive containers containing artificial saliva at 5 ± 3 °C and 60 ± 3 °C. The immersion time in each container was 15 s with a transfer time of 15 s between containers. A total of 40 specimens from 3 groups (VT, VTA, GD), making a total of 120 samples, were divided into 10 samples for each condition (n = 10) of thermal cycling: C0 - before thermal cycling; C1 3000 cycles; C2 - 6000 cycles; C3 - 10 000 cycles). Within the particle-reinforced GIC (VT), only VTA was selected for the thermal cycling test due to the best result obtained in the mechanical strength tests. The thermal cycling tests were carried out by immersing the samples in a Fusayama´s artificial saliva solution . The composition of the Fusayama saliva is shown in Table 2. The pH of the artificial saliva solution was approximately 5.5. 2.4. Microscopic and Chemical Analyses Two specimens of each group were prepared for field emission guns scanning electron microscopy (FEG-SEM). Specimens were wet-ground on SiC abrasive papers down to 1200 mesh. After griding, the specimens were cleaned in distilled water using an ultrasonic bath and then polished with a diamond (1 µm) paste. After preparation, the specimen´s surfaces were sputter coated with carbon to be analyzed by FEG-SEM (FEI NOVA 200; USA). The microstructure of these materials was analyzed before and after thermal cycling at magnifications between 200x and 10000x under secondary (SE) and backscattered electron (BSE) under voltage of 5-15 kV. The chemical analysis was performed in specific areas of the organic matrix and inorganic nano-particles by energy dispersive spectroscopy (EDAX Pegasus X4M; USA). 2.5. Statistical Analyses The results of the compressive tests of the different types of samples and after different thermal cycling conditions were analyzed by analysis of variance (ANOVA) using Origin software (8.5.1 OriginPro, OriginLab Corporation, MA, USA). Shapiro-Wilk Test assessed the normality of the population. The difference between the mean values for each group was considered statistically different when p < 0.05. The Tukey multiple comparisons test was used to compare the results with each other.
Effect of Zirconia and Alumina Fillers
The Open Dentistry Journal, 2016, Volume 10 61
Table 1. Information on the diferent materials used in this study: composition, particle size and weight. Material Glass ionomer (Vitremer, 3M, ESPE, USA) (VT)
Composition (% wt.) Liquid: Canforoquinone, HEMA, alquenoic acid, water (28%) Powder: fluoraluminumsilicate glass (SiO2, Al2O3, CaF2, AlF3,AlPO4,ZrO2 (72%)
Particle size (µm ou nm)
Comercial powder particles: 12.5 µm
Glass ionomer reinforced with Alumina (VTA1)
Liquid: Canforoquinone, HEMA, alquenoic acid, water (27.2%) Comercial powder particles: 12.5 µm Powder: fluoraluminumsilicate glass (68.9%), Nano-particles Al2O3 nano-fillers: < 50 nm (3.9%)
Glass ionomer reinforced with Alumina (VTA2)
Liquid: Canforoquinone, HEMA, alquenoic acid, water (26.8%) Comercial powder particles: 12.5 µm Powder: fluoraluminumsilicate glass (67.1%), Al2O3 NanoAl2O3 nano-fillers: < 50 nm particles (6.1%)
Liquid: Canforoquinone, HEMA, alquenoic acid, water (27%) Powder: fluoraluminumsilicate glass (68.3%), Al2O3 nanoparticles (4.7%)
Comercial powder particles: 12.5 µm ZrO2 nano-fillers: